HAL Id: hal-02315264
Submitted on 14 Oct 2019
HAL is a multi-disciplinary open access
archive for the deposit and dissemination of sci-entific research documents, whether they are pub-lished or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est destinée au dépôt et à la diffusion de documents scientifiques de niveau recherche, publiés ou non, émanant des établissements d’enseignement et de recherche français ou étrangers, des laboratoires publics ou privés.
Aging response investigation of 2017 Al alloy processed
by gravity and squeeze casting
Najib Souissi, Catherine Mabru, Chedly Bradai
To cite this version:
Najib Souissi, Catherine Mabru, Chedly Bradai. Aging response investigation of 2017 Al alloy pro-cessed by gravity and squeeze casting. International Journal of Materials Research, Carl Hanser Verlag GmbH & Co, 2019, 110 (9), pp.859-864. �10.3139/146.111806�. �hal-02315264�
an author's https://oatao.univ-toulouse.fr/24337
Souissi, Najib and Mabru, Catherine and Bradai, Chedly Aging response investigation of 2017 Al alloy processed by gravity and squeeze casting. (2019) International Journal of Materials Research, 110 (9). 859-864. ISSN 1862-5282
, Catherine Mabrub
, Chedly Bradaia
aUniversité de Sfax, Ecole Nationale d’Ingénieurs de Sfax (ENIS), LASEM, Tunisia bUniversité de Toulouse, Institut Clément Ader (ICA), ISAE, Toulouse, France
Aging response investigation of 2017 Al alloy
processed by gravity and squeeze casting
Suitable pressure levels and heat treatment of casting wrought aluminum alloy are key process parameters in making components with better metallurgical properties. For this purpose, the effect of applied pressure and aging treatment on the microstructure and the mechanical proper-ties of an industrial 2017 aluminum alloy manufactured by gravity and direct squeeze casting processes are investi-gated in this paper. After treating to various aging states, the correlation between these parameters and the character-istics of the cast alloy has been analyzed and discussed. Keywords: Squeeze pressure; 2017 Al alloy; Aging tem-perature; Microstructure; Mechanical properties
ties of squeeze cast 6061 Al alloy and found that the strength of the alloy decreases with the presence of the (FeCrMn)3SiAl12phase and increases with that of the finely
dispersed Mg2Si phase. Zhang et al.  reported that the
heat treatment caused an improvement of the tensile strength and elongation of SC Al–Cu based alloy. However, reports on aging temperature effect of SC wrought Al alloy are very few. It must be noted that precipitation behavior is known to have an important influence on the metallurgical properties of Al alloys.
Al-4 wt.%Cu (2xxx series) alloys are a precipitation hardening in which Cu promotes the formation of h-Al2Cu precipitates. The decomposition of the supersaturated solid solution (SSS) is believed to proceed in the following steps: SSS ? Guinier–Preston (GP) zones ? h’’ ? h’ ? h-Al2Cu
. Obviously, the development of high-performance al-loys requires a great understanding of the relationship be-tween processing parameters and mechanical properties through a quantitative prediction of the precipitation beha-vior. More specifically, wrought 2017 aluminum alloy, which is widely used in aircraft and aerospace structures [10, 11], has gained a growing interest in it especially when formed by the SC technique [12 – 15]. Moreover, it is re-ported that the combination of squeeze pressure and heat treatment offers several advantages that make wrought alu-minum alloys acquire improved mechanical properties [6, 8]. An understanding of the interrelationships between these parameters is particularly important since the me-chanical properties of casting components are highly corre-lated with the final microstructure and crystallographic tex-ture. Thus, the main objective of the present work is to investigate the effects of the aging temperature and to de-velop a suitable age-hardening heat-treatment process for gravity die casting (GC) and SC wrought 2017 Al alloy. It focuses on the relationship between the microstructure and the mechanical behavior of the material.
2. Experimental procedure
2.1. Material and specimen preparation
The casting experiments were conducted using a 2017 A aluminum alloy, which is widely used as wrought product in various mechanical areas [16, 17]. Its chemical composi-tion, as determined by spectral analysis, is shown in Ta-ble 1.
It was received as an extruded bar of diameter 80 mm and melted at 7008C in a graphite crucible using an electric resistance furnace. The casting process was carried out 1. Introduction
Among the different techniques described for materials forming, the squeeze casting (SC) process is used to pro-duce high integrity and low cost aluminum alloy . Dur-ing the solidification of the melt, the direct action of pres-sure activates two principal phenomena that are not generally observed in traditional die casting methods. First, the pressure generates a high cooling rate due to the reduc-tion of the air gap between the metal and the die wall, hence, there is a much larger effective contact area . In addition to that, the temperature of the liquidus could rise upon application of pressure, leading to a higher degree of undercooling . The change in the nucleation ratio and cooling rate would increase, which creates a finer grain size . The second phenomenon caused by SC is the fact that direct applied pressure inhibits defects associated with shrinkage cavities and porosity formation . This elimi-nates casting drawbacks and results in a better quality of casting products with a much higher density. On the other hand, heat treatment processing is considered as a promis-ing method to improve the quality of aluminum alloys. Yet, some research studies investigating the effect of heat treatment process on casting wrought Al alloys have been reported in literature [5 – 8]. In this regard, Kim et al.  studied the effect of aging times on the microstructure and mechanical properties of 7075 Al alloy. The results show that the fine-grained structures and the uniform distribution of eutectics at the periphery of the grain boundaries caused significant changes in hardness and tensile strength of spe-cimens. Skolianos et al.  assessed the influence of T6 heat treatment on the microstructure and tensile proper-Int. J.
through a solid mold and a punch made from heat treated H13 steel.
The direct SC experiments were conducted on a hydrau-lic press, where the pressure on the molten metal is kept at 90 MPa until the end of solidification. In GC, molten alloy was poured directly into the die without external pressure. The mold was preheated up to 2008C. The as-cast billets were rod-shaped; 23 mm in diameter and 110 mm in length. The choice of casting parameters was based on previous works [12 – 14]. Afterwards, the billets were solution trea-ted at 5008C for 8 h followed by water quenching. In order to investigate the effects of aging temperature and the ap-plied pressure on the microstructure and mechanical prop-erties, some quenched specimens were placed in the fur-nace (6 h) for the artificial aging process at different temperatures. Figure 1 shows an overall scheme of the ela-boration process and the experimental set-up followed in the present study.
2.2. DSC analyses
The differential scanning calorimetry (DSC) experiments were conducted on a SETARAM DSC-92 instrument for temperatures ranging from 25 to 6008C at a heating rate of 10 K min–1. The specimens were turned to disks of 4 mm
diameter and 6 mm high and placed in a hermetic alloy sealed aluminum capsule.
2.3. Microstructural characterization
The X-ray diffraction (XRD) measurements were per-formed using a Philips PW 1800 with Cu-Ka radiation.
The fracture surfaces of the tensile specimens were exam-ined with a JEOL 6460 LV scanning electron microscope (SEM).
2.4. Mechanical tests
Vickers microhardness (HV) tests were performed with a MEKTON hardness tester, at a load of 300 g applied for 30 s. Five measurements were taken at randomly selected points on the middle transverse section of the billet with a diamond pyramidal indenter. Tensile tests were carried out at room temperature using an MTS-810 universal testing machine with a crosshead speed 2 mm min–1. In order to
ensure the reproducibility of the tensile results, three tests were performed for each condition.
3. Results and discussion
The DSC thermograms and the Vickers microhardness measurements, as a function of aging temperature after water quenching of both GC and SC specimens, are plotted in Fig. 2. It is clearly shown that the microhardness of SC alloy is higher than those of the GC alloy. This is a result of the change in microstructure and the densification of an as-cast alloy caused by the applied pressure . The first in-tense exothermic signal centered at around 708C is as-signed to the formation of GP zones while the following weak endothermic peaks (around 858C) to their dissolution. The wide exothermic peak centered at 1708C is associated with h" phase precipitation. These metastable precipitates are responsible for the maximum microhardness values
Fig. 1. Experimental set up flowchart.
Table 1. Chemical composition of 2017 A aluminum alloy.
Elements Cu Mg Si Fe Mn Ni Pb Zn Cr Al
, and this is commonly observed at 1808C. It was also noticed that the h" peak of the SC (90 MPa) sample is larger than that of the GC (0 MPa), which is consistent with its higher microhardness. However, the wide exothermic peaks at 3208C are ascribed to the formation of incoherent h’ precipitates. Thus, the formation of the latter leads to a substantial decrease in microhardness . Added to that, the intense endothermic peaks at 5198C for GC and 528 8C for SC specimens are attributed to the melting of the inter-metallic compound h-Al2Cu . Moreover, the thermal
effects associated with h’ ? h transformation may not be sufficient to exhibit a separate signal during the DSC scans. As shown in Fig. 2b, this indicates that the peak relative to the melting of h phase is shifted toward higher temperatures with respect to that of GC specimen. This can be attributed
to the increase in eutectic temperature in correlation with the increase in pressure .
X-ray diffractograms of the three states of GC and SC samples are illustrated in Fig. 3. The XRD patterns of both cast alloys under 0 MPa (Fig. 3a) and 90 MPa (Fig. 3b) re-veal the Bragg reflections of the soluble Al2Cu and
insolu-ble Al12(Fe,Mn,Cu)3Si intermetallic phases. Other residual
phases are expected to be dissolved into the matrix by solu-tion treatment. These diffracsolu-tion results are consistent with those published by Birol [18, 20, 21]. It is also seen that the intensity of the diffraction peaks related to the Al2Cu
phase tends to broaden with aging temperature, confirming the reported precipitation sequence. This indicates that, during the aging process, the Cu separated out in the form of Al2Cu which are predominant precipitates in the alloy.
Fig. 2. (a) Microhardness variations and DSC thermograms of GC and SC specimens. (b) Magnification of the DSC curves showing the melting peaks of h phases.
Figure 4 presents the results of the SEM and EDX (energy dispersive X-ray) analysis of the sample aged at 1808C pre-pared by gravity and squeeze casting process, respectively. The SEM-image shows a wide intermetallic precipitation distributed among the grain boundaries, as already ob-served in the optical micrographs. Also, a lot of shrinkage microporosity is seen in gravity samples (Fig. 4a), while nearly no porosity is observed in squeeze casting samples (Fig. 4b). The predominant phases were identified by EDX (Fig. 4a’ and Fig. 4b’) analysis once again to be the h-Al2Cu intermetallic phases in both GC and SC samples
aged at 1808C.
The tensile properties such as ultimate tensile strength (UTS), yield strength (YS) and elongation percent (El%) of the GC and SC specimens in the different states I (quenched), II (quenched + aged 1808C) and III (quen-ched + aged 3208C) are compiled in Table 2. This shows that the GC specimens have low tensile properties than the SC specimens since the intensity of the applied pressure has a significant influence on the mechanical properties of the 2017 Al alloy [6, 13]. The effect of aging temperature on tensile properties showed that the aging temperature of 1808C (state II) presents the highest values of UTS and YS and the lowest value of El%. The enhancement of UTS and
Fig. 4. SEM images and corresponding EDX analysis of: (a, a’) gravity, and (b, b’) squeeze cast samples each aged at 1808C.
Table 2. Tensile properties results of the investigated alloy in the different metallurgical states.
Process Metallurgical state UTS(MPa) YS(MPa) El(%)
GC (0 MPa) I (quenched) 200 125 1.7 II (aged 1808C) 219 175 1.2 III (aged 3208C) 175 118 2.5 SC (90 MPa) I (quenched) 278 199 2.2 II (aged 1808C) 298 223 1.85 III (aged 3208C) 276 121 3.1
YSare likely due to the higher precipitates density of meta-stable Al2Cu and insoluble Al12(Fe,Mn,Cu)3Si precipitates.
These precipitates reduce the dislocation movement and thus a higher stress is required for its bowing. It is observed that the best combination of properties, i. e. high UTS (298 MPa) and YS (223 MPa), is achieved when aging and pressure are at 1808C and 90 MPa, respectively. In addition as expected, the El% varies inversely with the other tensile features. It is thus fair to conclude that the variation of ten-sile properties with squeeze pressure and heat treatment shows a good synchronized effect with microhardness mea-surements. This variation is the result of microstructural changes that have been observed previously.
Figure 5 shows typical fracture surfaces of the tensile specimens. On a macroscopic scale, the tensile fracture sur-face of the GC (0 MPa) specimens is at around 908 angle re-lative to the load direction for uniaxial tension, which is the characteristic of a brittle fracture surface. However, the SC
(90 MPa) specimens are considered to be ductile and typi-cally fail at approximately 458 with respect to the load di-rection of the uniaxial tension.
High magnification examination of the fracture surface of the GC specimens shows that the existence of micropor-osity (see arrows in GC) and the coarse grain size become the principal source of low ductility. This is a typical fea-ture of intergranular fracfea-ture paths. Obviously, with no ap-plied pressure, the alloy exhibits shrinkage problems asso-ciated with gas porosity due to the low interdendritic fluidity of the molten material . The tensile fracture sur-face of the SC specimens corresponds to transgranular frac-ture and reveals that microvoids mostly disappear and that equiaxed dimples occupy a large area. Inclusions and preci-pitates that initiate the ductile rupture are also observed in the fractography. However, the Al2Cu intermetallic
com-pounds that inevitably exist at the grain boundaries (see ar-rows in SC), lead to early fractures by creating notch effects
during the tensile test . It is also revealed that the break-age of intermetallic phases into smaller parts facilitates the dislocation motion. Generally, it can be concluded that the existence of cavities and higher density of precipitates is the principal source of lower ductility.
In this study, the effect of squeeze pressure combined with the artificial aging process on the microstructure and the mechanical properties of the cast 2017 A aluminum alloy have been quantified. The conclusions of this work can be summarized as follows:
1. Microhardness evolution of the investigated alloy at various aging temperatures shows that the microhard-ness increases at first and then decreases as aging tem-perature increases. The maximum and the minimum values are attained when aging at 1808C and 320 8C, re-spectively. In addition, the differential scanning calori-metry (DSC) analysis reveals the transformations of the different phases dissolved in the Al matrix.
2. After aging at 1808C, the microstructure of both SC and GC alloys was characterized by a high density of meta-stables precipitates, which corresponds to the maximum value of microhardness.
3. The rise of UTS, YS, microhardness and the fall of ducti-lity at an aging temperature of 1808C is more likely due to the precipitation of hard Al2Cu phase and the
elimina-tion of gas porosity by applied pressure. These results are in good agreement with the microstructural evolu-tion according to the different aging temperatures. 4. The examination via SEM fractography and elongation
results of both SC and GC alloys indicates that the frac-ture mode becomes more ductile at 3208C.
 B. Lin, W. Zhang, Z. Lou, D. Zhang, Y. Li: Mater. Des. 59 (2014) 10. DOI:10.1016/j.matdes.2014.02.012
 M.T. Abou El khair: Mater. Lett. 59 (2005) 894. DOI:10.1016/j.matlet.2004.11.041
 Z. Han, X. Huang, A.A. Luo, A.K. Sachdev, B. Liu: Scr. Mater. 66 (2012) 215. DOI:10.1016/j.scriptamat.2011.10.041
 A. Maleki, B. Niroumand, A. Shafyei: Mater. Sci. Eng. A 428 (2006) 135. DOI:10.1016/j.msea.2006.04.099
 T.M. Yue : J. Mater. Process. Technol. 66 (1997) 179. DOI:10.1016/S0924 0136(96)02516 2
 S.W. Kim, D.Y. Kim, W.G. Kim, K.D. Woo: Mater. Sci. Eng. A 304 306 (2001) 721. DOI:10.1016/S0921 5093(00)01594 X  S.M. Skolianos, G. Kiourtsidis, T. Xatzifotiou: Mater. Sci. Eng. A
231 (1997) 17. DOI:10.1016/S0921 5093(97)00067 1
 Z. Ming, Z. Wei wen, Z. Hai dong, Z. Da tong, L. Yuan yuan: Nonferr. Metal. Soc. 17 (2007) 496.
DOI:10.1016/S1003 6326(07)60122 8
 J. da Costa Teixeira, D.G. Cram, L. Bourgeois, T.J. Bastow, A.J. Hill, C.R. Hutchinson: Acta Mater. 56 (2008) 6109.
 K. Saï, L. Taleb, G. Cailletaud: Comput. Mater. Sci. 65 (2012) 48. DOI:10.1016/j.commatsci.2012.06.035
 G. Giuliano: Manuf. Letters. 10 (2016) 10. DOI:10.1016/j.mfglet.2016.08.003
 N. Souissi, S. Souissi, J. Lecompte, M.B. Amar, C. Bradai, F. Ha louani: Int. J. Adv. Manuf. Technol. 78 (2015) 2069.
DOI:10.1007/s00170 015 6792 0
 N. Souissi, S. Souissi, C.L. Niniven, M.B. Amar, C. Bradai, F. Ha louani: Metals 4 (2014) 141. DOI:10.3390/met4020141  N. Souissi, S. Souissi, C.L. Niniven, M.B. Amar, C. Bradai, F. Ha
louani: Int. J. Mater. Eng. Innovation 6 (2015) 59. DOI:10.1504/IJMATEI.2015.069801
 M.B. Amar, S. Souissi, N. Souissi, C. Bradai: Int. J. Microstruct. Mater. Prop. 7 (2012) 491. DOI:10.1504/IJMMP.2012.051229  C. Vargel: The most common wrought aluminum alloys. In corro
sion of aluminium; Elsevier, Amsterdam, The Netherlands (2004) 65 66. DOI:10.1016/B978 008044495 6/50009 4
 Metallic materials and elements for aerospace vehicle structures. Military: Handbook 5H., US Department of Defense, USA (1998).  Y. Birol: Mater. Sci. Eng. A 528 (2011) 5636.
 B. Zlaticanin, B. Radonjic, M. Filipovic: Mater. Sci. Forum 453 454 (2004) 193.
DOI:10.4028/www.scientific.net/MSF.453 454.193  Y. Birol: J. Mater. Proc. Technol. 211 (2011) 1749.
DOI:10.1016/j.jmatprotec.2011.05.016  Y. Birol: Mater. Chem. Phys. 131 (2012) 694.
 E. Hajjari, M. Divandari: Mater. Des. 29 (2008) 1685. DOI:10.1016/j.matdes.2008.04.012
 W. Dai, S. Wu, S. Lü, C. Lin: Mater. Sci. Eng. A 538 (2012) 320. DOI:10.1016/j.msea.2012.01.051
(Received December 24, 2018; accepted March 23, 2019; online since July 10, 2019)
Correspondence address Najib Souissi
Ravago Middle East Company Industrial city 2 Cross Road 308 & 315 PO BOX 10311, Jubail 35748 Saudi Arabia. Tel.: +966509279529 +21621134957 E mail: email@example.com firstname.lastname@example.org